M. Planak et al. Mjerenje kontaktnog trenja u obradama prostornog deformiranja
Tehniki vjesnik 19, 4(2012), 727-734 727
ISSN 1330-3651 UDC/UDK 621.9.01:620.178.16
POSSIBILITIES TO MEASURE CONTACT FRICTION IN BULK METAL FORMING Miroslav Planak, Zlatan Car, Marko Krulja, Dragia Viloti, Igor Kamarik, Dejan Movrin
Original scientific paper
Friction occurs in all metal forming operations and, in general, it has a negative impact on process parameters, die life, as well as workpiece quality. In cold metal forming processes high interface pressures between die and material take place. These pressures can be the limiting factor of application of cold forming. By reducing interfacial friction, contact pressures can be reduced too. Knowledge of friction amount (factor of friction and/or friction ratio m) is essential for calculation of the main process parameters (load, energy), for choosing a proper lubricant but also for numerical modelling of forming operations. There exist a number of experimental methods to determine friction in metal forming processes. Current paper deals with the possibilities to evaluate friction. It analyses and assesses a number of existing friction models in cold metal operations. Proposal of a new friction model for cold metal forming operations is presented and discussed. Measurement of friction force in backward extrusion for different lubrication conditions was also preformed. Keywords: cold backward extrusion, experimental tooling, friction models Mjerenje kontaktnog trenja u obradama prostornog deformiranja
Izvorni znanstveni lanak Trenje je neizbjena pojava u svim postupciima plastinog deformiranja metala i ima negativan utjecaj na parametre procesa, radni vijek alata, kao i kvalitetu radnog komada. U hladnom prostornom deformiranju veliki pritisci djeluju izmeu alata i radnog komada. Ovi pritisci mogu biti limitirajui faktor prilikom primjene tehnologija deformiranja. Smanjenjem kontaktnog trenja, smanjuju se i kontaktni pritisci. Poznavanje parametara trenja (faktora trenja i/ili omjera trenja m) je od velikog znaaja prilikom prorauna parametara procesa (npr. sila ili energija) i odabira odgovarajueg sredstva za podmazivanje, kao i numeriku simulaciju obrade. Postoje mnogobrojne metode za odreivanje parametara trenja u obradama deformiranjem. Neke od ovih metoda opisane su u ovom radu. Takoer je predstavljen i novi model za odreivanje parametara trenja u obradama deformiranjem. U radu je izvreno i mjerenje sile trenja u procesu protusmjernog istiskivanja za razliite vrste maziva. Kljune rijei: eksperimentalni alati, hladno protusmjerno istiskivanje, modeli trenja 1 Introduction
One of the important influential factors in all metal forming operations is friction which arises between the die and workpiece material. Friction increases load and energy requirement as well as die wear. Reduction of friction amount is therefore one of the main tasks in planning and realization of metal forming processes. It can be achieved by different measures: by selecting die materials that exhibit low adhesion (i.e. ceramics), by reducing roughness of the die surface, by subjecting die-workpiece interface to ultrasonic vibrations . But, in practical realization of metal forming operations the most effective and most employed way to reduce friction is lubrication of interfacial surfaces during deformation. There exist a wide range of different lubricants for metal forming processes whose function is not only to reduce friction but also to cool the die-workpiece contact, to reduce wear, to prevent cold welding and to control surface finish of the workpiece .
Knowledge of friction magnitude is needed for three reasons. First, forming load and energy requirement cannot be calculated without knowledge of friction. Second, in numerical analysis (i.e. finite element analysis) friction is an essential input parameter, and third, the amount of friction is the main criterion for the selection of lubricant .
Friction amount is quantified by a non-dimensional parameter: factor of friction () or/and friction ratio (m). Both friction indicators are obtained experimentally. For knowing (m), frictional shear stress f can be expressed as (Coulomb friction model):
f = p, 0 0,5 (0,577).
If there is no relative sliding at the die-workpiece
interface (in cases where pressure p is significantly higher than effective stress K: p>>K) frictional shear stress is determined as (Constant friction model): f = m max (2) m friction ratio, 0 m 1 max yield stress of the material in pure shear.
General friction model states that the frictional stress
is expressed by:
= f k (3) f friction factor expressing the friction in real contact (0 f 1) k shear flow stress, where k = max in expression (2) real to apparent contact area ratio.
In this model friction is proportional to normal stress at low pressures and fairly constant at high pressures as shown in Figure 1 .
For determination of non-dimensional parameter and m different experimental models have been developed. All of them simulate real metal forming processes such as sheet metal forming, extrusion, hot forging, cold forging, etc.
Possibilities to measure contact friction in bulk metal forming M. Planak et al.
728 Technical Gazette 19, 4(2012), 727-734
Figure 1 Friction stress in general friction model 
Current paper elaborates a number of most employed
friction models in cold bulk metal forming, including own model proposal for determination of factor of friction . Furthermore, friction force in backward extrusion of steel has been obtained experimentally, for different lubrication cases. For that reason special tooling was designed and made. 2 Models for measurement of friction in bulk metal forming
Great variety of metal forming processes differ from each other in terms of pressure, temperature, velocity, stress state, tribological conditions etc. Therefore, there is no universal friction model which would enable evaluation of friction conditions in all metal forming processes. Most of them are developed for specific operations.
Although tribological conditions during one metal forming operation change at certain contact point with time (and therewith changes also), most of the experimental models only enable determination of average value of and m.
In Tab. 1 some of the most applied experimental models for determination of friction in bulk metal forming are presented and evaluated.
Table 1 Models for friction assessment
Ring compression test Schema
Principle A ring-shaped billet is compressed by two plates in several increments. Deformation of diameter and height is measured after each increment. Friction is evaluated by comparing obtained results (curve) with friction calibration curves given in literature.
It is a very simple test. There is no need for load measurement or knowledge of material yield stress. This test is most suitable for processes with low effective strains.
New billet shape for ring compression test Schema
Principle The only difference between this test and conventional ring test is in the billets shape.
Original height/diameter proportions of conventional ring test are maintained.
This test is for processes where low nominal pressure and high friction is anticipated.
Forward bar extrusion Schema
Principle In this test cylindrical billet is extruded through conventional forward extrusion die. During observed interval, height h0 decreases to h01 and load FT decreases for FT. Load reduction FT is a function of only FC (other force components during this interval remain constant). Friction coefficient is a function of FT, die geometry and material yield stress.
This method can be used where more severe strains prevail. Forward bar extrusion test requires load measurement and knowledge of material yield stress.
Backward cup extrusion Schema
Principle In backward cup extrusion punch forces the billets material to flow sideways through the gap between the punch head and container. By measuring forces F1, F2 and Ff and by knowing tool/die geometry and material yield stress, friction can be calculated.
This test is most suitable for processes with high effective strains. Loads measurements, as well as material yield stress are needed.
M. Planak et al. Mjerenje kontaktnog trenja u obradama prostornog deformiranja
Tehniki vjesnik 19, 4(2012), 727-734 729
Backward extrusion with a twist Schema